# Shear Cracking of Prestressed Girders with High Strength Concrete

- Emad L. Labib
^{1}, - Y. L. Mo
^{1}Email author and - Thomas T. C. Hsu
^{1}

**7**:33

https://doi.org/10.1007/s40069-013-0033-4

© The Author(s) 2013

**Received: **25 December 2012

**Accepted: **11 February 2013

**Published: **29 March 2013

## Abstract

Prestressed concrete (PC) is the predominant material in highway bridge construction. The use of high-strength concrete has gained wide acceptance in the PC industry. The main target in the highway industry is to increase the durability and the life-span of bridges. Cracking of elements is one aspect which affects durability. Recently, nine 7.62 meter long PC I-beams made with different concrete strength were designed according to a simple, semi-empirical equation developed at the University of Houston (UH) (Laskar et al., ACI Journal 107(3): 330–339, 2010). The UH Method is a function of shear span-to-depth ratio (*a*/*d*), concrete strength \( \sqrt {{f}_{c}' } \), web area \( b_{w} d \), and amount of transverse steel. Based on testing these girders, the shear cracking strength of girders with different concrete strength and different shear span-to-depth ratio was investigated and compared to the available approaches in current codes such as ACI 318-11 (2011) and AASHTO LRFD Specifications (2010).

## Keywords

## 1 Introduction

The use of high strength concrete (HSC, i.e. concrete compressive strength \( {f}_{c}^{\prime } > 55\,{\text{MPa}} \)) has gained wide acceptance in the PC industry. Standardization in the design and manufacturing of the precast bridges has been optimized. Bridge superstructure elements such as the PC I-beams, double tee and box beams are generally plant-produced precast and PC products inheriting the advantages of durability, economy, low maintenance and assured quality. The most commonly used precast/PC beam for short-to-medium-spans is the I-beam. An I-beam consists of a top and a bottom flanges with a slender web joining the flanges. The bottom flange and some portion of the web-bottom are reinforced with prestressing strands (tendons); thus the bottom and top flanges build up the flexural strength. The web is reinforced with vertical/transverse deformed reinforcing bars (rebars), referred to as stirrups, which contributes towards the shear strength of the beam.

In the design of PC girders, an adequate margin of safety must be provided against both flexure and shear cracking under service load. Although cracking does not mean a structural failure, in the long term, cracking affects the durability of the structural element. It increases the environmental effects on the embedded steel. Moreover, cracks in general looks uncomfortable for public. Therefore, one of the most important criteria in designing concrete structure is to prevent cracking under the act of the different loads.

Cracking stress of a structural element in shear, which is the concern of this paper, does not depend on the amount of transverse steel. It depends only on the tensile strength of concrete. Most the current provisions, such as ACI Codes and AASHTO LRFD Specifications, calculate the tensile strength as a function in the concrete compressive strength \( {f}_{c}^{\prime } \). Rizkalla et al. (2009) conducted an experimental program to study material properties of PC members. Based on comparing the experimental results with AASHTO LRFD specifications, they found that the currently specified modulus of rupture might not be satisfied for high strength concrete. Perera and Mutsuyoshi (2011), concluded based on testing high strength concrete tension members that the average tensile strength for different concrete strength even higher than 100 MPa were between \( 0.32\sqrt {{f}_{c}^{\prime } } \) and \( 0.37\sqrt {{f}_{c}^{\prime } } \).

In general, the current code provisions were driven for normal concrete \( \left( {{f}_{c}^{\prime } < 55\,{\text{MPa}}} \right) \). The primary focus of this paper is to compare the current codes provisions of calculating the tensile strength in the web at shear cracking to that obtained from the experimental program presented later. The tested girders had different concrete compressive strengths and different transverse reinforcement ratios. The girders were also loaded using different shear span-to-depth ratios as will be discussed later.

## 2 Experimental Program

Nine girders were designed, cast, and tested to investigate the shear cracking strength of the web of PC I-girders. Girders had an effective depth of 611 mm and a web thickness of 76 mm. Girders had different concrete compressive strength. Because it is very difficult to measure stresses during experiments, an indirect method was used. The method depends on finding the stresses by knowing strains and the modulus of elasticity of concrete. As it will be discussed later, strains in the web was measured at each side by using a complete rosette of ten linear variable displacement transformers (LVDT). The modulus of elasticity for the different concrete was found by testing standard cylinders 152 × 304 mm. The compressive strain along the cylinders’ longitudinal axis was measured using 203 mm extensometer installed at the middle of the tested cylinders according to ASTM-C469 (2002).

## 3 Test Girders

Concrete mix proportions used for casting girders.

Materials kg/m | Group A | Group F | Group C |
---|---|---|---|

Cement type-III | 218 | 308 | 415 |

Fly ash type-F | 89 | 147 | 119 |

Cementitious content | 307 | 455 | 534 |

Fine aggregate | 685 | 685 | 634 |

Coarse aggregate | 1304 | 1125 | 1304 |

Coarse agg./fineagg. ratio | 1.91 | 1.64 | 2.06 |

Water | 107 | 136 | 142 |

Water/cement ratio | 0.49 | 0.43 | 0.34 |

Water/cementitious materials ratio | 0.35 | 0.30 | 0.27 |

Superplasticizer (mL/100 kg) | – | 624 | 832 |

Retarder (mL/100 kg) | – | 65 | 260 |

Slump (cm) | 16.5 | 21.6 | 26.7 |

Actual average strength (MPa) | 48.3 | 89.6 | 110.3 |

Several cylinders 150 × 300 mm were cast at the same time with each girder. The concrete was placed into each cylinder in three layers. Each layer was tapped with round rod 25 times. Then, cylinders was initially cured by keeping them covered under the same conditions as their girders.

Groups A and F girders had 14 seven-wire, low-relaxation prestressed straight tendons with a diameter of 13 mm, as a flexural reinforcement in the bottom flange. Group C girders had 14 seven-wire, low-relaxation prestressed straight tendons with a diameter of 13 mm oversized to increase the bending moment capacity ensuring shear failure of the girders. The prestressing tendons had a nominal tensile strength of 1,862 MPa. The locations of the prestressing tendons and different types of reinforcing steel in the tested girders are shown in Figs. 1 and 2.

^{o}angle, similar to the ACI Code. In Laskar et al. (2010), a more realistic concept of seeking a path of minimum shear resistance among a series of individual stirrups is used. The minimum number of stirrups intersecting the minimum shear resistance line at 45

^{o}is taken as \( [({d}/{s}) - 1] \). Thus,

Reinforcement Details for Modified Tx28 Girders (All dimensions are in mm).

Girder | Tendons | Mild steel reinforcement | |||||||||
---|---|---|---|---|---|---|---|---|---|---|---|

Nos. | Dia. | Transverse Steel (\( \phi \)16) “S”-rebar | Top flange flexural steel (\( \phi \)13) | Bottom flange flexural steel | |||||||

Sp. | Ratio (%) | Longitudinal direction | Lateral direction | Extra flexural steel | Confinement steel (\( \phi \)13) | ||||||

“T”-rebar | “A”-rebar | “C”-rebar | |||||||||

Nos. | Sp. | Nos. | Sp. | Nos. | Sp. | ||||||

A1 | 14 | 12.7 | 149 | 1.76 | 10 | 89 | 26 | 298 | – | 106 | 149 |

A2 | 14 | 12.7 | 114 | 2.30 | 10 | 89 | 34 | 229 | – | 138 | 114 |

F1 | 14 | 12.7 | 140 | 1.88 | 10 | 89 | 28 | 279 | – | 114 | 140 |

F2 | 14 | 12.7 | 102 | 2.58 | 10 | 89 | 38 | 203 | – | 154 | 102 |

F3 | 14 | 12.7 | 108 | 2.43 | 10 | 89 | 36 | 216 | – | 146 | 108 |

F4 | 14 | 12.7 | 79 | 3.31 | 10 | 89 | 32 | 248 | – | 196 | 83 |

C2 | 14 | 12.7 | 83 | 3.18 | 6 | 38 | 32 | 248 | 6 \( \phi \) 25 | 96 | 165 |

C3 | 14 | 12.7 | 76 | 3.44 | 10 | 89 | 27 | 305 | – | 100 | 152 |

C4 | 14 | 12.7 | 64 | 4.13 | 6 | 38 | 30 | 191 | 6 \( \phi \) 25 | 120 | 127 |

## 4 Test Set Up

The girder was positioned in the middle of this spacing width on top of two load cells placed at the north and south ends. The load cells of 2,224 KN capacity were placed on top of the steel pedestals fixed to the strong floor. On top of the load cells, bearing plates to support the girders were placed with a roller on the north end and a hinge on the south end, thus allowing the girder to rotate freely at the supports and to expand freely along its length. The actuators were provided with bracings for their lateral stability.

Actuator loads were applied through a roller assembly consisting of two 152 × 305 × 51 mm thick hardened steel bearing plates and two hardened steel rollers of 51 mm diameter and 305 mm in length. This ensured uniform and frictionless load transfer from actuators to the girder surface. The bearing plates and rollers were heat-treated to maximum possible hardness, to minimize local deformations. Lead sheets were used between the load bearing plates and girder surface to aid in uniform loading. The MTS “MultiFlex” System precisely controlled the applied loads and displacements through the actuators. Each girder was first loaded using Actuators B and C under a load-control mode at a rate of 9 KN/min. As soon as the slope of load versus displacement curve for girder being tested dropped, the actuator control-mode was switched to a displacement-control at a rate of 5 mm/h until shear failure occurred at either end of the girder. The displacement-control mode was essential in capturing the ductility or brittleness behavior of the girder failing in shear.

## 5 Instrumentations

Strains measured by the above discussed sensors and the applied loads by actuators as well as the shear forces at both ends of each girder measured by actuators and load cells respectively were monitored continuously and stored by the HBM “Spider-8” Data Acquisition System. Shear and flexure cracks formed on the girder during the load test regularly were marked on the grid. Shear crack widths were measured at different load intervals using a hand-held microscope having a 0.0254 mm measuring precision.

## 6 Test Results and Discussion

### 6.1 Experimental Modulus of Elasticity

Test variables and tensile strength at shear cracking of girders.

Beam I.D. | a/d | \( f_{c}^{\prime } \) (MPa) | (ρ %) | E (MPa) | \( f_{t} \) (MPa) | |
---|---|---|---|---|---|---|

A1 | 1.77 | 48.28 | 1.76 | 29,968 | North | 4.27 |

South | 3.60 | |||||

A2 | 3.00 | 49.66 | 2.30 | 30,295 | North | – |

South | 3.67 | |||||

F1 | 1.77 | 91.03 | 1.88 | 38,577 | North | 4.42 |

South | 4.65 | |||||

F2 | 3.00 | 89.66 | 2.58 | 38,336 | North | 3.8 |

South | 4.68 | |||||

F3 | 1.77 | 91.72 | 2.43 | 38,697 | North | 3.48 |

South | 3.64 | |||||

F4 | 2.25 | 90.34 | 3.31 | 38,457 | North | 4.61 |

South | 6.06 | |||||

C2 | 3.00 | 103.45 | 3.18 | 40,668 | North | 3.46 |

South | 4.07 | |||||

C3 | 1.77 | 116.55 | 3.44 | 42,742 | North | 5.13 |

South | 5.00 | |||||

C4 | 3.00 | 105.52 | 4.13 | 41,004 | North | 4.08 |

South | – |

Girder A2 was loaded using shear span-to-depth ration of 3.00. The LVDTs rosette was installed next to the loading points (actuators) as can be seen in Fig. 3. During the test, the north LVDT rosette missed measuring the tensile strains at the location of first shear crack which appeared out of the studied zone.

At the beginning of testing girder C4, the south actuator had a controlling problem which resulted in applying a huge sudden load which let the south end cracked before the starting of the test. Therefore, the tensile strains measured during the test at the south end did not considered in calculating the tensile stresses of the girder because they are not virgin readings.

Because the concrete is well known for its non-linear stress–strain curves. The initial stiffness of the stress–strain curve which represents the modulus of elasticity \( {\text{E}}_{\text{c}} \) was evaluated within the linear segment at the beginning of the stress–strain relationships. This linear segment is taken till the stress of 45 % of the ultimate compressive strength according to ACI 318-11 (2011). Vogel and Svecova (2012) took the initial stiffness till stress equals to 40 % of the ultimate strength of the tested cylinder.

### 6.2 Tensile Strain in Concrete at Shear cracking

According to the ACI 318-11 (2011), the shear cracks should start to appear in the web of prestressed I-girders if the principle tensile stress at the location of expected shear cracks exceeds \( 0.33\sqrt {{f}_{c}^{\prime } ({\text{MPa}})} \). Tamai et al. (1987) used \( 0.31\sqrt {{f}_{c}^{\prime } ({\text{MPa}})} \) as a limit for the tensile strength causing cracks in concrete. This approach was later used by Belarbi and Hsu (1995) to establish the smeared concept of smeared cracked of concrete under shear. National Cooperative Highway Research Program has tested ten full scale prestressed girders at University of Illinois (NCHRP 2007). They loaded the girders with a uniform distributed load till failure. They observed that the first crack was always a web shear crack. In most the cases this first web shear crack appeared at higher load than the cracking load \( V_{cw} \) specified in AASHTO Standard Specifications (2002). This experimental program could not evaluate the cracking load at different shear span-to-depth ratios because of using a uniform distributed load.

In this paper, the ACI 318-11 (2011) approach will be validated for different concrete strength. Therefore, the cracking tensile stresses of the test girders need to be evaluated. The easiest and the most accurate way to evaluate stresses in such specimens is to measure the corresponding strains, and by knowing the modulus of elasticity of used material, stresses can be evaluated.

The ultimate shear strength of the PC girders is known to be strongly affected by the shear span-to-depth ratio. This was obviously concluded from the experimental tests done before by many researchers such as Lyngberg (1976), Elzanaty et al. (1986), Robertson and Durrani (1987), Kaufman and Ramirez (1988), Shahawy and Batchelor (1996), and recently by Laskar et al. (2010). From Fig. 8 it can be concluded that the tensile strength causing shear cracks is not affected by the shear span-to-depth ratio used in loading the girders. It can be seen that the measured tensile strength at cracking using different shear span-to-depth ratios is comparable for the same concrete strength.

## 7 Conclusions

- 1.
The ACI 318-11 (2011) approach for calculating the modulus of elasticity is still valid for high strength concrete up to 117 MPa.

- 2.
The experimental results from this study shows that the ACI 318-11 (2011) approach of calculating the shear cracking strength of PC girders is still valid for high-strength concrete up to 117 MPa.

- 3.
The shear cracking strength of PC girders is not affected by the shear span-to-depth ratio or the amount of transverse steel.

## Declarations

### Acknowledgments

The research presented in this paper is financially supported by Texas Department of Transportation. The research findings presented in this paper are those from the authors, and they are not necessary to express the sponsor’s opinion.

### Open Access

This article is distributed under the terms of the Creative Commons Attribution License which permits any use, distribution, and reproduction in any medium, provided the original author(s) and the source are credited.

This article is published under license to BioMed Central Ltd.**Open Access**This article is distributed under the terms of the Creative Commons Attribution License which permits any use, distribution, and reproduction in any medium, provided the original author(s) and the source are credited.

## Authors’ Affiliations

## References

- AASHTO. (2002).
*Standard specifications for highway bridges*(17th ed.). Washington, DC: American Association of State Highway and Transportation Officials (AASHTO).Google Scholar - AASHTO. (2010).
*AASHTO LRFD bridge design specifications*(4th ed.). Washington, DC: American Association of State Highway and Transportation Officials (AASHTO).Google Scholar - ACI 363R-92. (1997). State-of-the-art report on high strength concrete. ACI Committee Report, pp. 55.Google Scholar
- ACI 318-11. (2011).Building code requirements for structural concrete. American Concrete Institute, Farmington Hills, MI: American Concrete Institute.Google Scholar
- ASTM-C469. (2002).
*Static modulus of elasticity and Poisson’s ratio of concrete in compression*. West Conshohocken, PA: ASTM International.Google Scholar - Belarbi, A., & Hsu, T. T. C. (1995). Constitutive laws of softened concrete in biaxial tension–compression.
*ACI Structural Journal,**92*(5), 562–573.Google Scholar - Carrasquiho, R. L., Nilson, A. H., & Slate, F. O. (1982). Properties of High Strength Concrete Subjected to Short-Term Loads. ACI Journal, Proceedings V. 78, No. 3, May–June 1981, pp. 171–178, and Discussion, Proceedings V. 79, No. 2, Mar–Apr. 1982, pp. 162–163.Google Scholar
- Elzanaty, A. H., Nilson, A. H., & Slate, F. O. (1986). Shear capacity of prestressed concrete girders using high-strength concrete.
*ACI Journal,**83*(3), 359–368.Google Scholar - Kaar, P. H., Hanson, N. W., & Capell, H. T. (1978). Stress-strain characteristics of high-strength concrete. Douglas McHenry International Symposium on Concrete and Concrete Structures, SP-55, American Concrete Institute, Detroit, 1978, pp. 161–185. Also, Research and Development Bulletin No. 051.01D, Portland Cement Association.Google Scholar
- Kaufman, M. K., & Ramirez, J. A. (1988). Re-evaluation of ultimate shear behavior of high-strength concrete prestressed I-girders.
*ACI Structural Journal,**85*(3), 295–303.Google Scholar - Laskar, A., Hsu, T. T. C., & Mo, Y. L. (2010). Shear strength of prestressed concrete beams part 1: Experiments and shear design equations.
*ACI Journal,**107*(3), 330–339.Google Scholar - Lyngberg, B. S. (1976). Ultimate shear resistance of partially prestressed reinforced concrete I-beams.
*ACI Journal,**73*(4), 214–222.Google Scholar - Martinez, S., NiIson, A. H., & Slate, F. O. (1982). Spirally-reinforced high-strength concrete columns. Research Report No. 82–10, Department of Structural Engineering, Cornell University, Ithaca, NY.Google Scholar
- NCHRP 579. (2007). Application of LRFD bridge design specifications to high-strength structural concrete: Shear provisions. NCHRP Report 579, Transportation Research Board, sponsored by ASSHTO and FHWA.Google Scholar
- Perenchio, W. F., & Khieger, P. (1978). Some physical properties of high strength concrete, Research and Development Bulletin No. RD056.01T, Portland Cement Association, Skokie, pp. 7.Google Scholar
- Perera, S. V. T. J., & Mutsuyoshi, H. (2011). Tension stiffening behavior of high-strength concrete tension members.
*Annual Research Journal of SLSAJ,**11*, 10–18.Google Scholar - Rizkalla, S., Zia, P., Mirmiran, A., Russell, H. G., & Mast, R. (2009). Proposal for concrete strength up to 124 MPa for bridge design. Journal of the Transportation Research Record, No. 2131, pp. 59–67.Google Scholar
- Robertson, I. N., & Durrani, A. J. (1987). Shear strength of prestressed concrete T girders with welded wire fabric as shear reinforcement.
*PCI Journal,**32*(3), 46–61.Google Scholar - Shahawy, M. A., & Batchelor, B. (1996). Shear behavior of full-scale prestressed concrete girders: Comparison between AASTHO specifications and LRFD code.
*PCI Journal, Precast/Prestressed Concrete Institute,**41*(3), 48–62.Google Scholar - Tamai, S., Shima, H., Izumo, J., & Okamura, H. (1987). Average stress–strain relationship in post yield range of steel bar in concrete. Concrete Library of JSCE, No. 11, June 1988, pp. 117–129. (Translation from Proceedings of JSCE, No. 378/Vol. 6, Feb 1987).Google Scholar
- Vogel, H. M., & Svecova, D. (2012). Evaluation of elastic modulus for high-strength concrete.
*ACI Materials Journal,**109*(M29), 313–322.Google Scholar